(Na,Ω)5[MnO2]13 does not have the romanèchite framework: a new tunnel structure determined and refined by EDT and synchrotron powder diffraction.
Mugnaioli, Enrico; Gemmi, Mauro; Merlini, Marco; Gregorkiewitz, Miguel; Acta Crystallographica, Section B 72 (2016) 893–903; doi:10.1107/S2052520616015651

data_2108440
_publ_contact_author_address
;
Dept of Physical, Earth and Environmental Sciences, University of Siena, 
via Laterina 8, I-53100 Siena, Italy
;
_publ_contact_author_email       gregormigu@gmail.com
_publ_contact_author_name        'M Gregorkiewitz'
_publ_contact_author_phone       +390577233810
_publ_section_title
;
 (Na,\W)5[MnO2]13 does not have the roman\`echite framework: a new tunnel
 structure determined and refined by EDT and synchrotron powder
 diffraction.
;
_publ_section_title_footnote     ' \W stands for 'vacancy''
_journal_coden_ASTM              ASBSDK
_journal_coden_Cambridge         1743
_journal_coeditor_code           DK5050
_journal_coeditor_notes          ' ?'
_journal_date_accepted           2016-10-04
_journal_date_from_coeditor      2016-10-04
_journal_date_printers_first     2016-10-13
_journal_date_proofs_in          2016-11-03
_journal_date_proofs_out         2016-10-13
_journal_date_recd_electronic    2016-07-14
_journal_issue                   06
_journal_name_full               'Acta Crystallographica, Section B'
_journal_page_first              893
_journal_page_last               903
_journal_paper_category          FA
_journal_paper_doi               10.1107/S2052520616015651
_journal_techeditor_code         B161565
_journal_techeditor_notes        ' ?'
_journal_volume                  72
_journal_year                    2016
_chemical_formula_moiety         Na3.94Mn13O26
_chemical_formula_sum            'Mn13 Na3.94 O26'
_chemical_formula_weight         1220.7
_space_group_IT_number           12
_space_group_name_Hall           '-C 2y'
_space_group_name_H-M_alt        'C 1 2/m 1'
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_audit_creation_method           'Jana2006 Version : 13/10/2015'
_cell_angle_alpha                90
_cell_angle_beta                 104.5992
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   22.6338
_cell_length_b                   2.8255
_cell_length_c                   14.9075
_cell_measurement_temperature    293
_cell_volume                     922.580
_computing_structure_refinement  'JANA2006 v 10-2015 EDT dynamical'
_computing_structure_solution    'SIR2011&Superflip on EDT intensities'
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.77
_diffrn_measured_fraction_theta_max 0.75
_diffrn_measurement_device       'TEM with beam precession'
_diffrn_measurement_device_type
' Zeiss Libra 120 equipped with Nanomegas Digistar P1000 precession'
_diffrn_radiation_probe          electron
_diffrn_radiation_type           electron
_diffrn_radiation_wavelength     0.0335
_diffrn_reflns_av_unetI/netI     0.0915
_diffrn_reflns_limit_h_max       30
_diffrn_reflns_limit_h_min       -30
_diffrn_reflns_limit_k_max       3
_diffrn_reflns_limit_k_min       -3
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            22736
_diffrn_reflns_theta_full        1.29
_diffrn_reflns_theta_max         1.35
_diffrn_reflns_theta_min         0.09
_exptl_absorpt_coefficient_mu    0
_exptl_crystal_density_diffrn    4.394
_exptl_crystal_density_meas      4.416
_exptl_crystal_density_method    rietveld
_exptl_crystal_description       cylinder
_exptl_crystal_F_000             1152
_exptl_crystal_size_max          0.000050
_exptl_crystal_size_rad          0.000020
_refine_diff_density_max         1.81
_refine_diff_density_min         -3.25
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_gt    2.10
_refine_ls_goodness_of_fit_ref   1.49
_refine_ls_number_constraints    0
_refine_ls_number_parameters     206
_refine_ls_number_reflns         6797
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.2389
_refine_ls_R_factor_gt           0.0665
_refine_ls_shift/su_max          0.0368
_refine_ls_shift/su_mean         0.0043
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     w=1/(\s^2^(F)+0.0001F^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0722
_refine_ls_wR_factor_ref         0.0860
_reflns_number_gt                2454
_reflns_number_total             6797
_reflns_threshold_expression     I>3\s(I)
_cod_data_source_file            dk5050sup12.cif
_cod_data_source_block           ROMANE_dyn_aniso
_cod_original_cell_volume        922.5801
_cod_database_code               2108440